Synthesis, characterization and disorder‒order phase transition of inorganic‒organic hybrid materials (H2dabco-CH2-Cl)[MIICl4] (M = Co, Zn)
Chen, Chun-Hong; Xu, Guan-Cheng; CrystEngComm 18 (2016) 550–; doi:10.1039/C5CE02059J

data_7223410
_publ_section_title
;
 Synthesis, characterization and disorder--order phase transition of
 inorganic--organic hybrid materials (H2dabco-CH2-Cl)[MIICl4] (M = Co, Zn)
;
_journal_issue                   4
_journal_name_full               CrystEngComm
_journal_page_first              550
_journal_paper_doi               10.1039/C5CE02059J
_journal_volume                  18
_journal_year                    2016
_chemical_formula_sum            'C7 H15 Cl5 N2 Zn'
_chemical_formula_weight         369.83
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-12-02 deposited with the CCDC.
2015-12-03 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 91.262(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.0664(17)
_cell_length_b                   12.075(2)
_cell_length_c                   11.0158(19)
_cell_measurement_reflns_used    8310
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.6312
_cell_measurement_theta_min      2.5030
_cell_volume                     1338.7(4)
_computing_cell_refinement       'Bruker SMART APEX II'
_computing_data_collection       'Bruker SMART APEX II'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0207
_diffrn_reflns_av_sigmaI/netI    0.0193
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            9301
_diffrn_reflns_theta_full        25.10
_diffrn_reflns_theta_max         25.10
_diffrn_reflns_theta_min         2.02
_exptl_absorpt_coefficient_mu    2.802
_exptl_absorpt_correction_T_max  0.5075
_exptl_absorpt_correction_T_min  0.4770
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.835
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             744
_exptl_crystal_size_max          0.31
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.28
_refine_diff_density_max         0.966
_refine_diff_density_min         -0.579
_refine_diff_density_rms         0.142
_refine_ls_extinction_coef       0.0061(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     140
_refine_ls_number_reflns         2353
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.059
_refine_ls_R_factor_all          0.0409
_refine_ls_R_factor_gt           0.0404
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0766P)^2^+15.2955P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1490
_refine_ls_wR_factor_ref         0.1494
_reflns_number_gt                2290
_reflns_number_total             2353
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5ce02059j2.cif
_cod_data_source_block           Zn100K
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7223407--7223410.cif.
;
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               7223410